Presentation on theme: "Metallurgy, Properties, Issues By Aldo M. Reti"— Presentation transcript:
1 Metallurgy, Properties, Issues By Aldo M. Reti PRECIOUS METALSMetallurgy, Properties, IssuesByAldo M. Reti
2 Topics: Metallurgical Aspects Gold Silver (Ag/Cu System), Reticulation Karat SystemLegal Aspects, HallmarkingColorDepletion Gilding, Gold LeafSilver (Ag/Cu System), ReticulationPlatinum (Pt Alloys)We will aim the focus on metallurgical perspective during this presentation.We will start with GoldFollow with SilverThen touch upon some important points about Platinum
3 Why “Precious”? Expensive, Rare, Desirable Noble Tradition, History GoldSilverPlatinumPGM (Platinum, Palladium, Iridium, Rhodium, Ruthenium, Osmium)Usually Alloyed, in order to enhance properties:MechanicalColor“Extend Use”
7 Colors of Gold Determined by Alloying Elements “Classic” System: Au/Cu/Ag (and Zn) is the basis for “Colored Golds”YellowRedGreen“White Golds”: Au/Cu/Ni or Au/Ag/Pd(Ni and Pd are very strong gold “whiteners”)
8 Gold Alloys What is Important? How much Gold?: Karat System Color PropertiesStrength, HardnessWorking CharacteristicsCastability (melting point, fluidity)(lost wax process, investment casting)
16 Isothermal projections defining the two phase regions in the Au-Cu-Ni ternary system
17 Au/Ni/Cu Pseudo-Binary Phase Diagrams at Constant Gold Contents
18 Color can be Measured! CIELAB Color System International System Adopted in 1976 by the International Committee on IlluminationASTM StandardClassic Example of Use: Paint Industry
19 CIELAB System Uses 3 Coordinates: L for Brightness (100=white, 0=black)a for Red-Green (100=red, -100=green)b for Yellow-Blue (100=yellow, -100=blue)Thus, Color can be represented by a vector in 3 coordinate space
20 These are called opponent colors because a human eye has only one variety of sensors (cones) for visualizing the red-green color pair. Thus, our eye will see either a tint of red or green, but not both at the same time. The most common color blindness is the red-green deficiency which is caused by this set of cones. Similarly, other sensors visualize yellow-blue or white-black components.
21 How to Measure Color? Spectrophotometer Manufacturers: Macbeth Hunter LaboratoriesBYK GardnerApplied Color Systems (ACS)
22 Examples of Color L a b Gold 84.0 4.8 34.3 Silver 95.8 -0.7 5.3 Copper70/30 Brass
23 Color Variation in 14 Kt Alloys Color Limits a Limits bRed > to 23.0Yellow -1.0 to to 23.0Green -1.0 to to 23.0White -1.0 to 1.0 less than 12.0
24 Color Difference Color of metal 1: L1, a1, b1 D2 = (L2-L1)2 + (a2-a1)2 + (b2-b1)2Human eye can differentiate D>2
26 Constant “L” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
27 Constant “a” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
28 Constant “b” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
29 Example of “Color Matching” Old piece of gold alloy needs to be matched (repaired) with a new 14Kt alloyMeasure color of old pieceSay, L = 93a = -4.5b = 19.5Now go to ternary charts to find composition of 14 Kt alloy with best match
30 Constant “L” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
31 Constant “a” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
32 Constant “b” Lines for 14 Kt Au/Cu/Ag/Zn Alloys
33 Best Color Match 14 Kt Alloy Silver: 70% x 41.67% = 29.17%Copper: 20% x 41.67% = %Zinc: % x 41.67% = %Gold: = 58.33%100.00%
34 Purple GoldPurple gold (also known as amethyst or violet gold) When gold and aluminium are alloyed in a certain fixed ratio, they form a gold intermetallic compound with the chemical formula AuAl2 (or Au6Al11). That is one atom of gold to two atoms of aluminium. This compound has an attractive purple color. In terms of composition, this compound is about 79% gold by weight and hence is hallmarkable as 18 carat gold.All intermetallic compounds, and purple gold is no exception, tend to be very brittle. They cannot be easily worked by conventional metal working processes. If one attempted to roll or hammer a piece of purple gold, it would shatter into pieces!“Purple Plague” when bonding gold wire to aluminum.
35 Blue Gold Au-Fe Alloys (i.e., 75 Au-25 Fe) Au-In Alloys Color Interference effect caused by thin film of oxide on surfacePurple films found in Tutankhamun gold (presence of Fe and As)
36 Depletion Gilding“Coloring the Gold”. Surface rich in gold. Remove base metals from the surface, which is enriched in gold.Process: conversion of base metals near the alloy surface:Chemical attack (alum and common salt), applied to Guanin (silver-rich). Form silver and copper chlorides, which at high temperature are absorbed by the crucible (cementation)Oxidation/leaching, applied to Tumbaga (copper-rich)Modern Method: Chemical “Bombing”Hot cyanide solution + hydrogen peroxide
37 Depletion Gilded Tumbaga from the Vicus Period, Peru Vicus period: from 400 BC to 100 AC.
38 Depletion GildingTribes in Pre-Columbian Peru, specifically the Moche and later the Chimu who were located in northern coastal Peru from between 250 BC to 600 AD and 800 AD to 1500 AD, respectively, hammered copper alloys to make ornamental objects. Pre-Columbian metalsmiths specialized in a copper alloy called tumbaga, which is primarily gold and copper, perhaps with some silver because silver typically occurs with gold when found in Andean stream beds. Tumbaga can achieve a gold color, despite being as low as twelve percent gold through a process called depletion gilding. Depletion gilding requires pickling a sheet of tumbaga in an acidic solution. Acidic pickling solutions could be easily obtained by the Moche and Chimu by soaking certain plant roots. The pre-Columbian Peruvian's primary interest in metalworking stems from a strong sense of spirituality. They believed that a divine power gave them the ability to "magically" make colors and designs appear in materials from where they had not previously existed, such as bringing a gold color out of a copper colored alloy. One can clearly see how the pre-Columbians would see depletion gilding a copper colored alloy and making it turn gold as a very spiritual activity since they did not understand the metallurgical principles behind depletion gilding.
40 9 Kt Gold-Silver Alloy treated 7 hours at 165 C in alum paste (x250)
41 9 Kt Gold-Silver-Copper Alloy after 9 cycles of torch heating in alum paste (x400)
42 Gold Leaf Few millionths of an inch thick (about 1/10 micrometers) Dates back….5,000 years? B.C., King TutankhamunMechanical method, no heat. Two dimensional tensional stresses and compression in the third directionGold with ~ 4% Silver. Also, some Copper (all have same crystal structure)Formation of new “sub-grains” as the gold alloy is workedDecorative uses, resistance to corrosion. Domes, altars, printing, buildingsBeating technique: Gold is first rolled into ribbons 1/1,000” thick, then cut into 1 1/4” squares and placed in squares of seaweed paper, encased in turn in parchment paper. This packet, called a “cutch”, is then squeezed in a press to compress the paper. The “cutch” is then beaten with a 17 lb hammer until the gold is in 4 inch squares. These are then placed in ox skins, coated with brime, a powder-like substance made from volcanic ash, brushed on with the hind leg of a Russian hare. This new packet, a “shoder” is beaten for 2 hours with a 9 lb hammer, then divided again into a “mould” wrapped in parchment paper, which is beaten with a 7 lb hammer. In all, about 82,800 blows are necessary to reduce the gold to 3 millionths of an inch in thickness. The gold is then so delicate that it can be cut only with a malacca reed shaped into a cutting tool or “wagon” which is slid across the gold. (From: The Gold Companion, by Timothy Green).
43 Corrosion of Gold Does Gold Tarnish? Tarnish: discoloration of metal surface caused by a thin layer of a reaction product (oxide or sulphide)Karat dependent, i.e., 14 Kt contains ~ 30 to 35 volume percent gold, the rest are base metalsAgents: perspiration, food, perfumes, household cleaners, etc. Also, solders are sometimes of lower karat
44 RESOURCES World Gold Council www.gold.org MJSA www.mjsainc.com Gold TechnologyGold BulletinMJSAAJM MagazineAnnual Trade ShowThe Santa Fe Symposium on Jewelry Manufacturing TechnologyInternational Precious Metals InstituteHallmarking OfficeFederal Trade CommissionThe Silver InstitutePlatinum Metals ReviewPlatinum Guild InternationalFEM (Institute for Precious Metals, Germany)Books:W.S. Rapson, “Gold Usage”, Academic Press (1978)A. Butts and C.D Coxe, “Silver, Economics, Metallurgy and Use”, Van Nostrand (1967)
45 Gold Filled Is it filled with gold? Early applications, wrapping gold around a metal rod, fusing it and drawn into wire
58 Gold Filled, Solder Core Wire made by “direct method”
59 Gold Filled, Solder Core Wire with a Nickel Interlayer
60 Intrinsic Value 14 Karat Gold: 14/24 x 400 = $ 233.33/oz 1/20 14 Kt G.F.: 1/20 x 14/24 x 400 = $ 11.67/oz1/20 12 Kt G.F.: 1/20 x 12/24 x 400 = $ 10.00/oz
61 U.S. Regulations for the Jewelry Industry National Gold and Silver Stamping Act (amended in 1976 with the Gold Labeling Act)Federal Trade Commission Guides for the Jewelry Industry (1997 revision)Guides cover industry products made of precious metals, diamonds, pearls, gemstones, watchcases and watchbands
62 FTC Guides Gold: minimum 10 Kt, 3 ppt tolerance Silver, Solid Silver, Sterling Silver:At least 92.5% Ag (925/1000)Coin Silver, 90.0% Ag (900/1000)Nickel Silver (German Silver)?
63 Gold FilledA product on which there has been affixed a plating of gold alloy of not less than 10 Kt finenessPlating must be at least 1/20 of the weight of the entire articlePlating must be affixed by mechanical means such as soldering, brazing, welding
65 Rolled Gold Plate, Gold Plate, Gold Overlay Same as Gold Filled, except the specified 1/20th by weightStrict marking requirements:1/40 12 Kt Gold Plate1/40 12 Kt R.G.P.1/40 12 Kt Gold OverlayCannot call it Gold Filled unless the plating is at least 1/20th by weight
66 Gold Electroplate Affix gold by electrolytic process No less than 10 KtMinimum thickness equivalent to 7 millionths of an inch (0.18 micrometers) of fine gold
67 Heavy Gold Electroplate As before, except coating with minimum thickness 100 millionths of an inch (2.5 micrometers)
68 Vermeil Base: Sterling Silver Minimum gold thickness: 120 millionths of an inch (3 micrometers)Gold coating either mechanical or electroplated
70 Quality MarkingTrademark: name or trademark of the manufacturer, importer, or sellerPlace trademark adjacent to quality markHowever……. System is difficult to police! and no Independent Assaying is Required
83 Microstructure of 0.010” thick Sterling Silver Strip, Solution Treated at 726C (x250)
84 Oxygen in Silver Silver Oxide is unstable at T>455 C (851 F) At One Atmosphere,Solubility of O in Ag above m.p.= 0.3%Solubility of O in Ag below m.p.= 0.006%“Spit”, Porosity, Oxides of base metalsAlso, oxygen diffuses very fast in solid silver
85 Deoxidation of Silver Carbon Reduction: C + O = CO Also, can use scavenger inert gas (Ar)In silver / copper alloys:C + Cu2O = 2Cu + COC + CuO = Cu + CO
86 Deoxidation of Sterling Silver After carbon reduction, add phosphorusGood scavenger, forms P2O5 (slag)Small amount, ~ 0.02%Add as “master alloy”: 85% Cu – 15% P
87 Reticulation Technique to apply “texture” Melt core of alloy, not the surfacei.e. 80Ag-20Cu, heat / chemically treatedOxidize the copper, then pickleSurface rich in Ag, higher melting pointMuch like depletion gilding!
93 Fire Stain or Fire Scale Results from annealing or heat treating silver / copper alloysTenacious, can be removed by picklingDevelopment of “alternative” Sterling Silver formulations, containing Zn, Sn, GeSome claim “anti-tarnish”Mixed Success…..Other elements have negative impact on mechanical properties. In summary, Ag/Cu is still the best combination!
94 Heishi American Indian Jewelry Heishi: Tiny beads from natural materials, hand made into precise sizes with a hole so they can be strung into necklacesSilver Heishi Beads, or liquid silver beadsMade from silver strip